Polymer Degradation and Stability 15 (1986) 33~6
Effect of Ozone on Rubbers: Countermeasures and Unsolved Problems*
P. M. Lewis
Tun Abdul Razak Laboratory, Malaysian Rubber Producers' Research Association, Hertford, Great Britain
(Received: 19 September, 1985)
Atmospheric ozone degrades polydiene rubbers by reacting with main chain unsaturation to cause chain scission and a diminished surface strength. When the rubber is exposed above a critical tensile strain, the degradation manifests itself as surface cracking which not only detracts from appearance but can also shorten the service life of a thin-walled product by initiating premature tensile or fatigue failure, by increasing stress relaxation and creep or by providing a pathway for fluid loss or ingress. Such attack may be reduced, or altogether prevented, by adding chemical antiozonants that diffuse to the surface to form a protective layer capable of reducing the rate of crack growth or, more usefully, of increasing the threshold strain above that in the exposed product.
The chemistry, physics and technology of ozone cracking and protection are reviewed with particular reference to natural rubber and to substituted p-phenylenediamine chemical antiozonants. Attention is also drawn to outstanding problems facing the rubber technologist and requiring further research by the chemist. Needs include a non-staining antiozonant capable of protection under dynamic, as well as static, exposure and protec- tive systems exhibiting improved resistance to wasteful loss caused by oxidation, volatilization and surface leaching by water and other fluids.
* Paper presented to Polymer Degradation Discussion Group meeting 'Polymer Stabilization and Degradation: Problems, Techniques and Applications', Manchester, Great Britain, ! 8-20 September, 1985.
33 Polymer Degradation and Stability 0141-3910/86/$03.50 Elsevier Applied Science Publishers Ltd, England, 1986. Printed in Great Britain
34 P. M. Lewis
By far the most damaging effect atmospheric ozone has on rubbers is the degradation of a stretched surface in such a way that a pattern of cracks forms (Fig. 1). Unlike sunlight crazing, which is random, ozone cracks grow perpendicularly to the direction of strain, and outdoors, in the absence of protection, they can appear within a few days at a typical ambient ozone concentration of 1-3 parts per hundred million parts (pphm) of air. In many cases this cracking is no more than superficial, without adverse effect on properties of the product. It assumes much greater importance when an unwanted crack triggers off more cata- strophic tear or fatigue failure, allows escape of a sealed fluid, increases stress relaxation or creep through a reduction in cross-sectional area, exposes components beneath a protective rubber surface and, not least, spoils the appearance of the product. Rubbers susceptible to ozone
Fig. 1. Ozone cracking in natural rubber. Left to right--looped triangular test piece (max. strain, ca 25%) stored in a cupboard for several years; a duplicate test piece exposed to ozonized air; a strip test piece (tensile strain, 20%) also exposed to ozonized air. Each of these samples contains a protective system unsuited to the conditions of
exposure used (see text).
Effect of ozone on rubbers 35
attack are those having main chain unsaturation. The handful of diene- based rubbers in this category account for over 90% of annual elastomer consumption. Most in need of protection are the general-purpose materials of natural rubber and its synthetic counterpart polyisoprene (I), polybutadiene (II) and the copolymers of butadiene and styrene (SBR--III). Also lacking ozone resistance are the oil-resistant copoly- mers of butadiene and acrylonitrile (nitrile rubber--IV). Some inherent stability is shown by polychloroprene (V) and much more by the predominantly saturated copolymer of isobutene and isoprene (butyl rubber--VI), but these, too, sometimes need the benefit of extra protection.
.~- -CH2~H=CH- -CH2- -~ (II)
.... fP ~ (III)
.~ [CH2---CH=CH~CH2]-~-5~ z CH2--CH~L;~,yo (IV)
...-..--CH 2~C==C H~ H 2~ (V)
[ CH 3 ] [ (~H3]
.~-]-C H 2 ---C=CH~C H 2~L-~-CH~C~-[ ~ (VI)
"~ L CH319~97~
The rubber industry has devised various protective measures, some of them very effective, but all with shortcomings. Because of the rubbers involved there is a sizeable market for antiozonants, which are used at higher concentrations than other antidegradants normally are. Addi- tional demands come from the hurdle of having to meet a specification, perhaps unrelated to service conditions, and the concern some end-users have that cracking, however unimportant, might just occur. One recent
36 P.M. Lew/s
forecast suggests that, whereas the EEC consumption of rubber chemi- cals will increase by 29% between 1982 and 1988, that of antidegradants, including antiozonants, will rise by 40%.
The purpose of this paper, which is intended for a non-specialist readership, is to review the methods available for combating ozone attack, highlight recent advances and identify the outstanding problems concerning both stabilization and testing.
A brief account of the generally accepted mechanism of ozone attack is instructive because cracking is a physico-chemical phenomenon, with its severity depending on the mechanical conditions of exposure (see Fig. 2), as well as the reactivity of the base polymer. For a more detailed treatment attention is drawn to a recent review by Razumovskii and Zaikov.
Rate of crack growth before coalescence
t ~ zone cracking
Light crazing . . . . . . . . . . . . . . . . . . . . . . . .
Threshold A Tensile strain strain
Log rate of b crack growth
Mechanical A Maximum fatigue strain "~
Fig. 2. Strain dependence of ozone cracking. (a) Static strain exposure. Note that, unlike ozone cracking, light crazing occurs independently of extension and is compara- tively shallow. (b) Dynamic strain exposure. Note that ozone attack is the only cause of crack growth below the mechanical fatigue limit of the rubber. For a soft natural
rubber vuicanizate the fatigue limit is typically ca. 70% extension.
Effect of ozone on rubbers 37
The ozonolysis of unsaturated rubbers has been shown to be complex, not least in natural rubber where naturally occurring non-rubber constituents can also participate, but there is some agreement with the Criegee mechanism 2 depicted below.
\0\3 ~C===:C~ 4- 0 3 ) /C---C\ (VII)
f / (VIII)
peroxides; 1 lactones; esters /t~ ~\
The key reactions are the initial addition of ozone across a main chain double bond to form the unstable molozonide (VII) and the subsequent chain scission caused by rearrangement of the intermediate zwitterion (VIII). In unstretched solid rubber such degradation is confined to a thin surface layer 3 (typically 0.5ltm thick) mainly because, unlike elemental oxygen, ozone reacts so rapidly with a double bond that none is available for penetration into the rubber bulk. The attack, however, can be sufficient to cause occasional 'frosting' (a white bloom-like appearance) on transparent and coloured surfaces (Fig. 3), and recently links have been drawn between ozone attack and loss in building tack 4 and decrease in ease of adhesion to polyester cordsS upon atmospheric storage of unvulcanized rubber mixes.
In most diene rubbers the ozone-degraded surface layer is mechanically extremely weak, often resembling a viscous liquid rather than a solid. Rupture of the layer in the vicinity of a stress-raising flaw of the type always present in a vulcanizate surface will expose virgin rubber and crack growth will commence.
38 P. M. Lewis
Fig. 3. 'Frosting' in natural rubber. In an unprotected transparent vulcanizate this effect causes loss in clarity because of a bloom-like appearance. Left to right-- unexposed; exposed for 3 days at 50 pphm ozone, with bottom part then wiped with acetone; exposed indoors in diffused daylight for 2 years. The test pieces are unstrained.
Definitive work by Braden and Gent, 6 using a fracture mechanics approach, identified two characteristic parameters for the development of ozone cracks under static strain conditions. In summary, these are as follows.
First, crack growth does not occur until a minimum tearing energy introduced by extending the rubber is exceeded. In the absence of stabilizers this threshold energy is substantially independent of ozone concentration and is broadly similar for all diene rubbers. In practical terms it corresponds to a threshold tensile strain of 3-5%, depending on stiffness.
Secondly, once the threshold condition is exceeded, a single isolated crack grows at an approximately constant rate independent of strain and in direct proportion to the ozone concentration. It is here that differences exist among rubber types. The rate in butyl rubber is an order of magnitude below that in natural rubber and SBR, not because of low unsaturation but because of high internal hysteresis. Raise the
Effect of ozone on rubbers 39
test temperature or add a plasticizer, and the rate increases to the natural rubber level because of greater chain mobility. The resistance shown by polychloroprene is attributed to double bond stabilization by the chlorine atom.
In plane rubber surfaces crack growth is strain dependent. 7 Just above the threshold value there will be few large enough flaws at the pre- requisite t